Transcript of "Optimization of tensile strengths response of plantain fibres"
1.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012 Optimization of Tensile Strengths Response of Plantain Fibres Reinforced Polyester Composites (PFRP) Applying Taguchi Robust Design C. C. Ihueze1, E. C. Okafor1*, A. J. Ujam2 1. Department of Industrial and Production Engineering, Nnamdi Azikiwe University, Awka, Nigeria 2. Department of mechanical/production engineering, Enugu State University of Science and Technology, Enugu, Nigeria * E-mail of the corresponding author: cacochris33@yahoo.comAbstractThis study focuses on the use of control factors(volume fraction of fibers (A), aspect ratio of fibers (B) and fibersorientation (C)) to determine the optimum tensile strength of plantain fibers reinforced polyester resin. Tensile testswas conducted on the replicated samples of plantain empty fruit bunch fiber reinforced polyester composite(PEFB)and plantain pseudo stem fiber reinforced polyester (PPS) respectively using Archimedes principles in each case todetermine the volume fraction of fibers. To obtain the optimum properties a Monsanto tensometer were used conducttensile tests to establish the control factor levels quality characteristics needed to optimize the mechanical propertiesbeing investigated. Taguchi robust design technique was applied for the greater the better to obtain the highest signalto noise ratio (SN ratio) for the quality characteristics being investigated employing Minitab 15 software. Theoptimum values of the control factors are established for empty fruit bunch composites and for pseudo stem fibercomposite. The empty fruit bunch fiber reinforced polyester matrix composite has the optimum tensile strength of40.28MPa , while the pseudo stem plantain fiber reinforced matrix composite has the tensile strength of 30.51MPa.The properties studied depend greatly on the reinforcement combinations of control factors and the composites ofempty fruit bunch are stronger in tension than that of pseudo stem.Key Words: composite matrix, plantain fibers, tensile strength, pseudo-stem, empty fruit bunch. Taguchi.1. IntroductionTensile strength of plantain fiber reinforced polyester composites is the maximum stress the material will bear whenit is subjected to a stretching load. The facts that composites in general can be custom tailored to suit individualrequirements have desirable properties in corrosive environment; provide higher strength at a lower weight and havelower life-cycle costs has aided in their evolution (Abdalla et al., 2008). It provides a good combination inmechanical property, thermal and insulating protection. Binshan et al., (1995) observed that these qualities inaddition to the ability to monitor the performance of the material in the field via embedded sensors give compositesan edge over conventional materials. Plantains (Musa spp., AAB genome) are plants producing fruits that remainstarchy at maturity (Marriot and Lancaster, 1983; Robinson, 1996) and need processing before consumption. Plantainproduction in Africa is estimated at more than 50% of worldwide production (FAO, 1990; Swennen, 1990).Nigeria is one of the largest plantain producing countries in the world (FAO, 2006). Plantain fiber can be obtainedeasily from the plants which are rendered as waste after the fruits have ripened. So plantain fiber can be explored as apotential reinforcement.Many investigations have been made on the potential of the natural fibers as reinforcements for composites and inseveral cases the result have shown that the natural fiber composites own good stiffness, but the composites do notreach the same level of strength as the glass fiber composite (Oksman and Selin, 2003). It was then realized that thefull economic and technical potential of any manufacturing process can be achieved only while the process is runwith the optimum parameters. Taguchi technique is a powerful tool for the design of high quality systems (Taguchi 62
2.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012and Konishi, 1987; Taguchi, 1993). The Taguchi approach enables a comprehensive understanding of the individualand combined from a minimum number of simulation trials. This technique is multi – step process which follow acertain sequence for the experiments to yield an improved understanding of product or process performance(Basavarajappa et al, 2007).In the present work polyester was used as a matrix material and plantain fibers used as reinforcing material toproduce a composite material to evaluate the various mechanical properties like Tensile strength (TS), at differentreinforcement combination to achieve the optimum strength.2. Literature/Background of StudyWith the growing global energy crisis and ecological risks, natural fibers reinforced polymer composites and theirapplication in design of equipment subjected to impact loading have attracted more research interests due to theirpotential of serving as alternative for artificial fiber composites (Bledzki, Sperber and Faruk, 2002; Mishra et al,2004). Many studies had been carried out on natural fiber likes kenaf, bamboo, jute, hemp, coir, sugar palm and oilpalm (Arib et al. 2006; Khairiah & Khairul 2006; Lee et al. 2005; Rozman et al. 2003; Sastra et al. 2005). Thereported advantages of these natural resources includes low weight, low cost, low density, high toughness, acceptablespecific strength, enhanced energy recovery, recyclability and biodegradability (Lee et al. 2005; Myrtha et al. 2008;Sastra et al. 2005). This study seeks to design and manufacture a natural fiber based composite at optimal levels ofmaterial combination to achieve maximum strength while maintaining earlier established properties.According to Derek (1981), many factors must be considered when designing a fiber-reinforced composite such as:Fiber length and diameter: the strength of a composite improves when the aspect ratio (L/D) is large, where L: fiberlength and D is the diameter of the fiber. The amount of fiber: the strength and stiffness of the composites increasewith increasing the volume fraction; Orientation of fibers: the orientation of fibers has a great role in the strength ofthe composites. One of the unique characteristics of fiber-reinforced composites is that their properties can betailored to make different types of loading conditions and this study aims at exploiting this inclination to achieve anoptimal design specification for materials subjected to dynamic working conditions.3. Material and MethodsThe methodology of this study employs traditional and experimental design methods of Taguchi method to optimizethe tensile, strength of plantain fiber reinforced polyester composite.3.1 Plantain fiber extraction and Chemical treatmentThe plantain fiber was mechanically extracted from both stem and empty fruit bunch. The fibers were soaked in a 5%NaOH solution for 4 hours, alkali treatment is a chemical method which can change the constituents of fibers. Thefibers were further treated with a solution of water and methanol (Saline treatment) in the ratio of 4:6 and thenneutralized with dilute acetic acid in the ratio of 100:10 and finally washed with water. The resultant fibers weredried at 30oC for 72 h before the examination of the tensile test. 63
3.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012 (a) Plantain stem fiber (b) Plantain empty Fruit Bunch Fiber Figure 1: Depiction of plantain fibers types3.2 Determination of fiber Volume Fraction through Archimedes principleCalculations of volume fraction of plantain fiber is achieved following the derivations from rule of mixtures based onthe procedures of (Jones 1998; Barbero 1998) and implementation of Archimedes procedures.3.3 Sample formation and determination of mechanical propertiesFlat unidirectional arrangements of the fibers were matted using natural rubber latex as the bonding agent. They werearranged to a thickness of 1.2mm and dried at room temperature for 72 hours. The composite manufacturing methodadopted for is based on open molding Hand lay-up processing technology in which the plantain fiber reinforcementmat is saturated with resin, using manual rollout techniques of (Clyne and Hull, 1996) to consolidate the laminateand removing the trapped air. A mild steel mold of dimensions (130×120×5) mm was used for casting thecomposites in a matching group of 10, 30 and 50% volume fractions and 10, 25, 40 mm/mm aspect ratio based ondesign matrix of table 2. At the time of curing, a compressive pressure of 0.05MPa was applied on the mould and thecomposite specimens were cured for 24 hours.Replicate samples of plantain fiber reinforced polyester matrix were then subjected to tensile tests using HounsfieldMonsanto Tensometer. The plantain stem and empty fruit bunch fiber reinforced composites were prepared for tensiletest in according to ASTM D638. Tests were carried out in Hounsfield tensometer model –H20 KW with magnificationof 4:1 and 31.5kgf beam force. The cross head speed is 1 mm/min. Each specimen was loaded to failure. The force -extension curve was plotted automatically by the equipment. The ultimate tensile strength and elastic modulus of thesamples were thereafter determined from the plot.3.4 Design of experiments (DOE) and Degree of Freedom (DOF) rulesTaguchi Robust design technique was applied for greater the better option of signal to noise ratio (eq. 11) using themeasured properties as quality characteristics and choosing three factor levels (Low, medium, high). The computedSN ratio for the quality characteristics were evaluated and optimum control factor levels established for theparameters. The signal to noise ratio condenses the multiple data points within a trial, depends on the type ofcharacteristics being evaluated. The S/N ratio for maximum tensile strength which comes under larger is bettercharacteristic, was calculated as logarithmic transformation of the loss function as shown in (2) (Ross, 1993). Thevariance of quality characteristics is measured as mean squared deviation MSD as expressed in (1). 64
4.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012According to the rule that degree of freedom for an orthogonal array should be greater than or equal to sum of chosenquality characteristics, (DOF) can be calculated by the formula of (3) expressed as(DOF)R = degree’s of freedom, P = number of factors, L = number of levels(DOF)R = 3(3 – 1) = 6Therefore, total DOF of the orthogonal array (OA) should be greater than or equal to the total DOF required for theexperiment. Thus L9 orthogonal array was selected and applied; the selection of orthogonal array depends on threeitems in order of priority, viz, the number of factors and their interaction, number of levels for the factors and thedesired experimental solution or cost limitation. A total of 9 experiments were performed based on the run ordergenerated by the Taguchi model. The model response is tensile strength; in the orthogonal array, first column isassigned to Volume fraction (%), second column is assigned to Aspect Ratio (lf/df), and third column is assigned toFiber orientations (± degree). The objective of the model is to maximize the tensile strength of PFRP.4. Discussion of ResultsIn this study the tensile strength of plantain fiber reinforced polyester were investigated for optimum reinforcementcombinations to yield optimum response employing Taguchi methodology. The signal to noise ratio and meanresponses associated with the dependent variables of this study are evaluated and presented. Traditionalexperimentation on replicated samples of empty fruit bunch fiber reinforced polyester composite were used toobtain the value of quality characteristics of tensile strength using different levels of control factors as in table1. The response tables for means and SN ratios shows that the volume fraction has the highest contribution ininfluencing the composite tensile strength, followed with fiber orientation as depicted in table 5 and figure 2-5.Table 1: Experimental outlay and variable sets for mechanical propertiesS/N PROCESSING FACTORS LEVEL 1 2 3 UNIT OBSERVED VALUE1 A: Volume fraction 10 30 50 %2 B: Aspect Ratio (lf/df) 10 25 40 mm/mm Tensile Strength,3 C: Fiber orientations ±30 ±45 ±90 Degree 65
5.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012Table 2 and table 3 show Taguchi DOE orthogonal array and Design matrix implemented for the larger the bettersignal to noise ratio (SN ratio).Table 2: Applicable Taguchi Standard Orthogonal array L9Experiment Parameter 1:A Parameter 2:B Parameter 3:C Parameter 4:DNumber1 1 1 1 12 1 2 2 23 1 3 3 34 2 1 2 35 2 2 3 16 2 3 1 27 3 1 3 28 3 2 1 39 3 3 2 1The tensile test signal -to-noise ratio for plantain empty fruit bunch fiber reinforced polyester composite is calculatedwith (2) using values of various experimental trials and presented as in table 3 so that for first experiment,Equation (1) is used in the computation of the mean standard deviation MSD as recorded in the following tables. 66
6.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012Table 3: Experimental design matrix for tensile test using composite made from plantain empty fruit bunchfiber reinforced polyester composite (ASTM-638)Expt. A: B: Aspect C: Fiber Specimen replicates tensile response (MPa) Mean Volume Ratio orientations ultimateNo. fraction (lf/df)(mm) (± degree) Trial 1 Trial2 Trial 3 tensile MSD SNratio (%) response (MPa)1 10 10 30 19.24679487 21.79487179 20.52083333 20.52083 0.002393 26.210332 10 25 45 18.92628205 18.84615385 18.88621795 18.88622 0.002804 25.522863 10 40 90 21.74679487 20.03205128 20.88942308 20.88942 0.002299 26.383884 30 10 45 23.79807692 25.30448718 24.55128205 24.55128 0.001662 27.79335 30 25 90 34.51923077 32.37179487 33.44551282 33.44551 0.000896 30.47786 30 40 30 25.000000 22.75641026 23.87820513 23.87821 0.001762 27.540837 50 10 90 31.33012821 34.93589744 33.13301282 33.13301 0.000916 30.379458 50 25 30 37.72435897 37.17948718 37.45192308 37.45192 0.000713 31.469029 50 40 45 28.23717949 28.86217949 28.54967949 28.54968 0.001227 29.11098The tensile test signal-to-noise ratio for plantain pseudo-stem fiber reinforced polyester composite is calculated with(2) using values of various experimental trials and presented as in table 4 so that for first experiment,Similarly, Equation (1) was utilized in the computation of the mean standard deviation MSD and recorded in table 4. 67
8.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012 8 3 2 1 37.28365 31.43012 9 3 3 2 31.5625 29.97899A standard approach to analyzing these data would be to use the analysis of variance (ANOVA) to determine whichfactors are statistically significant. But Taguchi approach uses a simpler graphical technique to determine whichfactors are significant. Since the experimental design is orthogonal it is possible to separate out the effect of eachfactor. This is done by looking at the control matrix, table 5 and calculating the average SN ratio ( ) and mean( ) responses for each factor at each of the three test levels as follows:For factor A average responsesA is at levels 1 in experiment 1, 2 and 3 so that the average responses are obtained asA is at levels 2 in experiment 4, 5 and 6 so that the average responses are obtained asA is at levels 3 in experiment 7, 8 and 9 so that the average responses are obtained asFor factor B average responsesB is at levels 1 in experiment 1, 4 and 7 so that the average responses are obtained as 69
9.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012B is at levels 2 in experiment 2, 5 and 8 so that the average response are obtained asB is at levels 3 in experiment 3, 6 and 9 so that the average responses are obtained asFor factor C average responsesC is at levels 1 in experiment 1, 6 and 8 so that the average responses are obtained asC is at levels 2 in experiment 2, 4 and 9 so that the average responses are obtained asC is at levels 3 in experiment 3, 5 and 7 so that the average responses are obtained as 70
10.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012This procedure is also followed in the computation of response for mean of PPS. The above computations were thenimplemented in Minitab 15 software and the results are presented in tables 6 and 7. Figures 2-5 are the excel graphicsfor SN ratio and mean tensile strength of plantain empty fruit bunch and pseudo stem fiber reinforced compositesbased on Larger is better quality characteristics.Table 6: Response Table for SN ratio and mean tensile strength of plantain empty fruit bunch fiber reinforcedcomposites based on Larger is better quality characteristicsResponse Signal –to- Noise Ratios Means of quality characteristicLevel A: Volume B:Aspect C:Fiber A: Volume B:Aspect C:Fiber Ratio Orientations (± Ratio Fraction (%) (lf/df) degree) Fraction (%) (lf/df) Orientations (± degree)1 26.85 29.85 29.60 22.54 31.67 30.782 30.19 29.52 28.19 32.79 31.85 26.523 30.93 28.60 30.18 35.40 27.21 33.43Delta 4.08 1.25 1.99 12.85 4.64 6.90Rank 1 3 2 1 3 2 71
11.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012Table 7: Response Table for SN ratio and mean tensile strength of plantain pseudo stem fiber reinforcedcomposites based on Larger is better quality characteristicsResponse Signal -to -Noise Ratios Means of quality characteristicsLevel A: Volume B:Aspect C:Fiber A: Volume B:Aspect C:Fiber Ratio Ratio Fraction (%) (lf/df) Orientations Fraction (%) (lf/df) Orientations ± degree) ± degree)1 26.04 28.13 28.41 20.10 26.07 27.282 28.60 29.16 27.48 27.29 29.93 24.003 30.32 27.68 29.08 33.04 24.44 29.16Delta 4.28 1.48 1.60 12.95 5.49 5.16Rank 1 3 2 1 2 3The average SN ratios and mean of means of the response tables are plotted against test levels for each of the threecontrol parameters. In figure 2-5 it is found that factor A which is the volume fraction of fibers has a stronger effecton SN ratios and mean of means than the other two control factors and hence more significant than other two controlfactors. 72
12.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012Figure 2: Main effect plots for signal-noise ratio-PEFB Figure 3: Main effect plots for means ratio-PEFBFigure 4: Main effect plots for signal-noise ratio-PPS Figure 5: Main effect plots for means-PPS4.2 Estimation of expected tensile responses based on optimum settingsAccording to Radharamanan and Ansui (2001), the expected response is estimated using the optimum control factorsetting from the main effects plots; by employing the response table for signal to noise ratio and the response tablefor mean, the expected response model is as in equation (4): (4)Where, EV= expected response, AVR = average response, Aop t = mean value of response at optimum setting offactor A, Bop t = mean value of response at optimum setting of factor B, Cop t = mean value of response at optimumsetting of factor C, So that for the empty fruit bunch and from figures 2 and 3 and table 5: 73
13.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012The expected responses is similarly computed for pseudo stem and presented in table 8. As a result of plots of figures2-5 one can conclude that the optimal settings of control parameters are as presented in table 8Table 8: Optimum setting of control factors and expected optimum strength of compositesComposite and property Control factor Optimum Optimum setting Expected optimum level strengthEmpty fruit bunch /tensile A 3 50 40.28MPa B 1 10 C 3 90Pseudo stem/tensile A 3 50 38.51 MPa B 2 25 C 3 904.3 Regression model for optimum tensile strengthTENSILE STRENGHT (Pseudo Stem) = 15.7 + 0.324A - 0.054B + 0.0505C (5)Table 9: Regression analysis for plantain pseudo stem fiber reinforced compositesPredictor Coef SE Coef T PConstant 15.684 4.876 3.22 0.024A: Volume fraction (%) 0.32365 0.08221 3.94 0.011B: Aspect Ratio (lf/df) -0.0543 0.1096 -0.50 0.641C: Fiber orientations (± degree) 0.05047 0.05265 0.96 0.382S = 4.02732 R-Sq = 76.9% R-Sq(adj) = 63.1%TENSILE STRENGHT (EFB) = 20.5 + 0.321A - 0.149B + 0.0693C (6)Table 10: Regression analysis for plantain empty fruit bunch fiber reinforced compositesPredictor Coef SE Coef T PConstant 20.507 6.237 3.29 0.022A: Volume fraction (%) 0.3213 0.1051 3.06 0.028B: Aspect Ratio (lf/df) -0.1486 0.1402 -1.06 0.338C: Fiber orientations (± degree) 0.06931 0.06735 1.03 0.351S = 5.15122 R-Sq = 69.7% R-Sq(adj) = 51.6% 74
14.
Innovative Systems Design and Engineering www.iiste.org ISSN 2222-1727 (Paper) ISSN 2222-2871 (Online) Vol 3, No 7, 2012Figure 6: Residual plots of tensile strength SN Ratio for plantain Pseudo stem and plantain empty fruit bunch fiberreinforced composites The coefficient of determination (R-Sq) is the proportion of variability in a data set that is accounted for by a statistical model of 5 and 6, it indicates that the predictors explain 76.9% and 69.7% of the variance in Tensile strength of plantain fiber reinforced composites when reinforcement is Pseudo stem and Empty fruit bunch respectively. The plots of fig 6 include a run order plot, a lag plot, a histogram, and a normal probability plot. A residual plot is a graph that shows the residuals on the vertical axis and the independent variable on the horizontal axis. If the points in a residual plot are randomly dispersed around the horizontal axis, a linear regression model is appropriate for the data; otherwise, a non-linear model is more appropriate. The residual plot shows a fairly random pattern, this random pattern indicates that a linear model provides a decent fit to the data. The data look fairly linear, although there might be a slight curve in the middle. Overall, linear regression is appropriate for these data at this level. 5. Conclusions The mechanical properties of plantain fiber reinforced polyester matrix composite (PFRP) have been extensively studied with following deductions: 1. The empty fruit bunch fiber reinforced polyester matrix composite has the optimum tensile strength of 40.28MPa when the control factors (volume fraction of fibers, aspect ratio of fibers and fibers orientation) are set 50%, 10 and 90 degree respectively, while the pseudo stem plantain fiber reinforced matrix composite has the tensile strength of 38.51MPa when the control factors (volume fraction of fibers, aspect ratio of fibers and fiber orientation) are set 50%, 25 and 90 degree respectively. 2. The properties studied depend greatly on the reinforcement combinations of control factors. 3. The composites of empty fruit bunch are stronger in tension than that of pseudo stem. 6. References Abdalla F. H., Megat M. H., Sapuan M. S. and B. B. Sahari (2008). determination of volume fraction values of filament wound glass and carbon fiber reinforced composites. ARPN Journal of Engineering and Applied Sciences. VOL. 3, NO. 4, pp. 7-11 Acott, Chris (1999). "The diving "Law-ers": A brief resume of their lives.". South Pacific Underwater Medicine Society journal 29 (1) pp 39-42. ASTM D3171 "Fiber content of resin-matrix composites by matrix digestion". Basavarajappa, S., G. Chandramohan, J.P. Dawim, (2007). Application of Taguchi techniques to study dry sliding wear behavior of metal matrix composites, Materials and design, 28: 1393-1398. 75
15.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Vol 3, No 7, 2012Binshan S. Y., Alrik L. Svenson and Lawrence C. Bank. (1995). Mass and Volume Fraction Properties of Pultruded Glass Fiber-Reinforced Composites. Research Report, Composites Volume 26 Number 10, Elsevier Science Limited, U.K.Box GEP, Hunter WG, Hunter JS. (1978). Statistics for experimenters. New York: Jhon Wiley and Sons.; 291–334.Box, G.E.P.; Hunter, J.S. (1957). Multi-factor experi-mental design for exploring response surfaces, Annals of Mathematical Statistics 28: 195-241. Cambridge University Press, Cambridge.Clyne, T. W. and Hull, D. (1996). An Introduction to Composite Materials, 2nd ed.Derek Hall, (1981) "An introduction to composite material", Cambridge University pressFood and Agriculture Organization. (1990). Production Yearbook 1990. FAO, Rome.Food and Agriculture Organization. (2006). Production Yearbook 2004. FAO, Rome.Jones R. M. (1998). Mechanics of composite materials. 2nd Ed. Edwards Brothers, Ann Arbor. Montgomery, D.C. (2009). Design and Analysis of Ex-periments; 7th edition. Hoboken, NJ: Wiley.Mishra, S. K. and Singh, V. P.:(2004). Long-term hydrological simulation based on the Soil Conservation Service curve number, J. Hydrol. Process., 18, 1291–1313,Oksman, K., M and J.F. Selin, (2003). Natural fibers as reinforcement in polylactic acid (PLA) composites. J. Comp. S. Skrivars ci. Technol., 63, pp 1317-1324.Radharamanan, R and Ansuj, A.P (2001), “Quality Improvement of a Production Process using Taguchi Methods”, Proceedings of Institute of Industrial Engineers Annual conference, Dallas, Texas, May 20-22, 2001, Paper Solutions.Robinson J.C (1996). Bananas and Plantains. CAB International, UK. pp. 238Swennen R (1990). Plantain cultivation under West African Conditions: A reference Manual. Int. Inst. Trop. Agric., Ibadan , Nigeria. pp. 24Taguchi, G. (1993). Taguchi on Robust Technology Development: Bringing Quality Engineering Upstream. ASME. New York.Taguchi, G. and Konishi, S., (1987). Orthogonal Arrays and Linear Graphs , American Supplier Institute Inc., Dearborn, MI. 76
16.
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. Prospective authors ofIISTE journals can find the submission instruction on the following page:http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar
Be the first to comment